#------------------------------------------------------------------------------
#$Date: 2016-03-24 01:58:58 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179549 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/18/4501896.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4501896
loop_
_publ_author_name
'Wang, Xiu-li'
'Hu, Hai-liang'
'Tian, Ai-xiang'
_publ_section_title
;
 Influence of Transition Metal Coordination Nature on the Assembly of
 Multinuclear Subunits in Polyoxometalates-Based Compounds
;
_journal_issue                   11
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              4786
_journal_paper_doi               10.1021/cg1006742
_journal_volume                  10
_journal_year                    2010
_chemical_formula_sum            'C12 H20 Ag3 Mo12 N16 O40 P S4'
_chemical_formula_weight         2662.54
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.000(5)
_cell_angle_beta                 109.803(5)
_cell_angle_gamma                90.000(5)
_cell_formula_units_Z            2
_cell_length_a                   9.609(5)
_cell_length_b                   21.569(5)
_cell_length_c                   14.079(5)
_cell_measurement_temperature    293(2)
_cell_volume                     2745.4(18)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0248
_diffrn_reflns_av_sigmaI/netI    0.0290
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            13585
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.80
_exptl_absorpt_coefficient_mu    3.976
_exptl_absorpt_correction_T_max  0.451
_exptl_absorpt_correction_T_min  0.417
_exptl_absorpt_correction_type   numerical
_exptl_crystal_colour            'dark red'
_exptl_crystal_density_diffrn    3.221
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2496
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.20
_refine_diff_density_max         1.073
_refine_diff_density_min         -1.402
_refine_diff_density_rms         0.126
_refine_ls_extinction_coef       0.00146(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.042
_refine_ls_hydrogen_treatment    refo
_refine_ls_matrix_type           full
_refine_ls_number_parameters     481
_refine_ls_number_reflns         4835
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.042
_refine_ls_R_factor_all          0.0405
_refine_ls_R_factor_gt           0.0330
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0082P)²+18.4966P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0624
_refine_ls_wR_factor_ref         0.0650
_reflns_number_gt                4223
_reflns_number_total             4842
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg1006742_si_002.cif
_cod_data_source_block           compound1
_cod_original_sg_symbol_H-M      P21/n
_cod_database_code               4501896
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ag1 Ag -0.15712(6) -0.05900(2) 0.47876(4) 0.04534(15) Uani 1 1 d . . .
Ag2 Ag 0.5000 0.0000 0.5000 0.0923(4) Uani 1 2 d S . .
P1 P 0.0000 0.0000 0.0000 0.0305(5) Uani 1 2 d S . .
Mo1 Mo 0.37303(5) -0.04163(2) 0.14267(3) 0.02419(12) Uani 1 1 d . . .
Mo2 Mo 0.17350(6) 0.06527(3) 0.24213(4) 0.04247(17) Uani 1 1 d . . .
Mo3 Mo 0.28880(6) 0.10947(3) 0.03597(4) 0.04443(18) Uani 1 1 d . . .
Mo4 Mo 0.21288(6) -0.08736(3) -0.11542(5) 0.04314(17) Uani 1 1 d . . .
Mo5 Mo 0.08889(6) -0.15620(3) 0.07213(4) 0.04223(17) Uani 1 1 d . . .
Mo6 Mo -0.0695(3) -0.0489(4) 0.2222(4) 0.0231(10) Uani 0.50(2) 1 d P A 1
Mo6' Mo -0.0806(3) -0.0739(5) 0.2017(4) 0.0247(12) Uani 0.50(2) 1 d P A 2
S1 S -0.1081(3) 0.21686(9) 0.40568(17) 0.0616(5) Uani 1 1 d . . .
S2 S 0.3197(3) 0.22749(9) 0.65438(16) 0.0740(7) Uani 1 1 d . . .
N1 N -0.3179(6) 0.0667(3) 0.4033(4) 0.0440(13) Uani 1 1 d . . .
N2 N -0.1856(6) 0.0449(2) 0.4408(4) 0.0385(12) Uani 1 1 d . . .
N3 N -0.0824(6) 0.0899(2) 0.4506(4) 0.0352(12) Uani 1 1 d . . .
C1 C -0.1603(7) 0.1413(3) 0.4165(4) 0.0340(14) Uani 1 1 d . . .
C5 C 0.4135(9) 0.1696(3) 0.6162(4) 0.0462(18) Uani 1 1 d . . .
N6 N 0.3720(6) 0.1143(2) 0.5772(4) 0.0389(13) Uani 1 1 d . . .
N7 N 0.4951(6) 0.0894(3) 0.5651(4) 0.0449(14) Uani 1 1 d . . .
N8 N 0.6075(7) 0.1257(3) 0.5957(5) 0.0587(17) Uani 1 1 d . . .
O1 O -0.0153(7) 0.0246(3) 0.1072(5) 0.0181(15) Uani 0.50 1 d P . .
O2 O -0.0521(7) -0.0665(3) 0.0367(5) 0.0197(15) Uani 0.50 1 d P . .
O3 O 0.1221(7) -0.0422(3) 0.0241(5) 0.0209(15) Uani 0.50 1 d P B .
O4 O 0.1433(7) 0.0151(3) 0.0679(5) 0.0210(15) Uani 0.50 1 d P . .
O5 O 0.3169(6) 0.0011(2) 0.2355(3) 0.0550(14) Uani 1 1 d . . .
O6 O 0.3954(6) 0.0401(2) 0.0858(3) 0.0540(14) Uani 1 1 d . . .
O7 O 0.3542(6) -0.0670(2) 0.0033(3) 0.0545(14) Uani 1 1 d . B .
O8 O 0.2749(6) -0.1132(2) 0.1496(4) 0.0539(14) Uani 1 1 d . . .
O9 O 0.2489(6) 0.1138(2) 0.1670(3) 0.0527(13) Uani 1 1 d . . .
O10 O -0.2265(8) -0.0722(4) 0.0929(5) 0.026(2) Uani 0.502(8) 1 d P . 1
O11 O -0.2031(8) 0.0248(3) 0.2052(6) 0.025(2) Uani 0.502(8) 1 d P . 1
O13 O 0.0462(8) -0.1036(4) 0.1841(5) 0.025(2) Uani 0.502(8) 1 d P A 1
O14 O 0.0772(8) 0.0007(4) 0.3018(6) 0.026(2) Uani 0.502(8) 1 d P A 1
O10' O -0.2575(9) -0.1123(4) 0.1003(6) 0.027(2) Uiso 0.498(8) 1 d P . 2
O11' O -0.1992(8) 0.0023(4) 0.1493(6) 0.027(2) Uiso 0.498(8) 1 d P . 2
O13' O 0.0222(8) -0.1437(4) 0.1906(6) 0.027(2) Uiso 0.498(8) 1 d P A 2
O14' O 0.0776(8) -0.0204(4) 0.2444(7) 0.026(2) Uani 0.498(8) 1 d P A 2
O12 O 0.1466(7) -0.1502(2) -0.0371(4) 0.0577(15) Uani 1 1 d . . .
O15 O -0.0051(8) 0.1140(5) 0.2335(9) 0.024(3) Uani 0.50(2) 1 d P . 1
O15' O -0.0042(8) 0.0905(5) 0.1806(10) 0.028(3) Uani 0.50(2) 1 d P . 2
O16 O -0.1203(9) -0.1821(7) 0.0061(6) 0.030(4) Uani 0.51(2) 1 d P . 1
O16' O -0.0923(9) -0.1414(7) 0.0017(6) 0.026(4) Uani 0.49(2) 1 d P . 2
O17 O 0.5402(11) -0.0761(18) 0.1935(15) 0.038(6) Uani 0.53(6) 1 d P B 1
O17' O 0.5515(13) -0.0423(16) 0.2184(13) 0.028(6) Uani 0.47(6) 1 d P B 2
O18 O 0.2581(6) 0.0907(3) 0.3593(3) 0.0706(18) Uani 1 1 d . . .
O19 O 0.4138(6) 0.1649(2) 0.0575(5) 0.0719(18) Uani 1 1 d . . .
O20 O 0.2986(5) -0.1329(3) -0.1727(4) 0.0661(17) Uani 1 1 d . B .
O21 O 0.1340(6) -0.2289(2) 0.1090(4) 0.0667(16) Uani 1 1 d . . .
O22 O -0.1205(4) -0.0877(2) 0.3078(3) 0.0350(10) Uani 1 1 d . . .
N4 N -0.3037(6) 0.1273(2) 0.3882(4) 0.0378(12) Uani 1 1 d . . .
C2 C -0.4323(8) 0.1675(4) 0.3463(6) 0.057(2) Uani 1 1 d . . .
H2A H -0.3999 0.2090 0.3409 0.068 Uiso 1 1 calc R . .
H2B H -0.4905 0.1671 0.3899 0.068 Uiso 1 1 calc R . .
H2C H -0.4910 0.1527 0.2806 0.068 Uiso 1 1 calc R . .
C3 C 0.0896(9) 0.2171(3) 0.4706(5) 0.0501(18) Uani 1 1 d . . .
H3A H 0.1333 0.1824 0.4472 0.060 Uiso 1 1 calc R . .
H3B H 0.1311 0.2549 0.4541 0.060 Uiso 1 1 calc R . .
C4 C 0.1285(10) 0.2128(3) 0.5829(5) 0.057(2) Uani 1 1 d . . .
H4A H 0.1033 0.1716 0.5995 0.068 Uiso 1 1 calc R . .
H4B H 0.0681 0.2422 0.6038 0.068 Uiso 1 1 calc R . .
N5 N 0.5570(8) 0.1771(3) 0.6272(4) 0.0584(18) Uani 1 1 d . . .
C6 C 0.6546(12) 0.2305(4) 0.6652(9) 0.117(5) Uani 1 1 d . . .
H6A H 0.7515 0.2212 0.6634 0.141 Uiso 1 1 calc R . .
H6B H 0.6609 0.2392 0.7334 0.141 Uiso 1 1 calc R . .
H6C H 0.6155 0.2660 0.6236 0.141 Uiso 1 1 calc R . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N3 Ag1 N6 131.33(19) 3_556 3_556
N3 Ag1 N2 114.24(18) 3_556 .
N6 Ag1 N2 114.02(19) 3_556 .
N7 Ag2 N7 180.00(14) . 3_656
O4 P1 O4 180.0(8) . 3
O4 P1 O3 122.8(4) . 3
O4 P1 O3 57.2(4) 3 3
O4 P1 O3 57.2(4) . .
O4 P1 O3 122.8(4) 3 .
O3 P1 O3 180.0(6) 3 .
O4 P1 O1 71.2(3) . .
O4 P1 O1 108.8(3) 3 .
O3 P1 O1 72.1(3) 3 .
O3 P1 O1 107.9(3) . .
O4 P1 O1 108.8(3) . 3
O4 P1 O1 71.2(3) 3 3
O3 P1 O1 107.9(3) 3 3
O3 P1 O1 72.1(3) . 3
O1 P1 O1 180.0(6) . 3
O4 P1 O2 71.7(4) . 3
O4 P1 O2 108.3(4) 3 3
O3 P1 O2 71.7(4) 3 3
O3 P1 O2 108.3(4) . 3
O1 P1 O2 97.9(3) . 3
O1 P1 O2 82.1(3) 3 3
O4 P1 O2 108.3(4) . .
O4 P1 O2 71.7(4) 3 .
O3 P1 O2 108.3(4) 3 .
O3 P1 O2 71.7(4) . .
O1 P1 O2 82.1(3) . .
O1 P1 O2 97.9(3) 3 .
O2 P1 O2 180.0(5) 3 .
O17' Mo1 O17 27.4(4) . .
O17' Mo1 O5 92.1(10) . .
O17 Mo1 O5 112.8(11) . .
O17' Mo1 O8 113.0(10) . .
O17 Mo1 O8 92.2(11) . .
O5 Mo1 O8 96.0(2) . .
O17' Mo1 O6 92.1(9) . .
O17 Mo1 O6 110.2(9) . .
O5 Mo1 O6 86.49(19) . .
O8 Mo1 O6 154.5(2) . .
O17' Mo1 O7 110.8(8) . .
O17 Mo1 O7 93.0(10) . .
O5 Mo1 O7 153.8(2) . .
O8 Mo1 O7 86.83(19) . .
O6 Mo1 O7 80.30(18) . .
O17' Mo1 O3 176.0(7) . .
O17 Mo1 O3 150.3(14) . .
O5 Mo1 O3 91.7(2) . .
O8 Mo1 O3 67.8(2) . .
O6 Mo1 O3 86.9(2) . .
O7 Mo1 O3 65.3(2) . .
O17' Mo1 O4 149.2(13) . .
O17 Mo1 O4 175.5(10) . .
O5 Mo1 O4 67.0(2) . .
O8 Mo1 O4 92.2(2) . .
O6 Mo1 O4 65.4(2) . .
O7 Mo1 O4 86.9(2) . .
O3 Mo1 O4 32.7(2) . .
O18 Mo2 O15' 117.6(5) . .
O18 Mo2 O9 103.4(3) . .
O15' Mo2 O9 92.8(3) . .
O18 Mo2 O5 99.4(2) . .
O15' Mo2 O5 141.8(5) . .
O9 Mo2 O5 87.4(2) . .
O18 Mo2 O15 90.4(4) . .
O15' Mo2 O15 27.1(3) . .
O9 Mo2 O15 99.6(3) . .
O5 Mo2 O15 166.3(3) . .
O18 Mo2 O14 87.3(3) . .
O15' Mo2 O14 84.9(3) . .
O9 Mo2 O14 168.9(3) . .
O5 Mo2 O14 87.8(3) . .
O15 Mo2 O14 83.2(3) . .
O18 Mo2 O14' 110.4(3) . .
O15' Mo2 O14' 85.3(4) . .
O9 Mo2 O14' 142.8(3) . .
O5 Mo2 O14' 72.3(3) . .
O15 Mo2 O14' 95.4(3) . .
O14 Mo2 O14' 26.3(3) . .
O18 Mo2 O1 157.4(3) . .
O15' Mo2 O1 48.4(5) . .
O9 Mo2 O1 95.6(2) . .
O5 Mo2 O1 93.5(2) . .
O15 Mo2 O1 74.2(4) . .
O14 Mo2 O1 74.7(3) . .
O14' Mo2 O1 56.2(3) . .
O19 Mo3 O6 104.3(2) . .
O19 Mo3 O10' 91.1(4) . 3
O6 Mo3 O10' 107.6(3) . 3
O19 Mo3 O10 117.3(3) . 3
O6 Mo3 O10 88.5(3) . 3
O10' Mo3 O10 28.9(3) 3 3
O19 Mo3 O16' 112.3(5) . 3
O6 Mo3 O16' 141.3(5) . 3
O10' Mo3 O16' 84.3(3) 3 3
O10 Mo3 O16' 85.7(3) 3 3
O19 Mo3 O9 98.7(3) . .
O6 Mo3 O9 86.7(2) . .
O10' Mo3 O9 160.3(3) 3 .
O10 Mo3 O9 143.7(3) 3 .
O16' Mo3 O9 76.1(3) 3 .
O19 Mo3 O16 87.5(4) . 3
O6 Mo3 O16 164.8(4) . 3
O10' Mo3 O16 81.3(3) 3 3
O10 Mo3 O16 94.6(3) 3 3
O16' Mo3 O16 25.0(3) 3 3
O9 Mo3 O16 82.0(3) . 3
O19 Mo3 O2 154.9(2) . 3
O6 Mo3 O2 100.3(2) . 3
O10' Mo3 O2 76.5(3) 3 3
O10 Mo3 O2 57.8(3) 3 3
O16' Mo3 O2 45.6(5) 3 3
O9 Mo3 O2 87.7(2) . 3
O16 Mo3 O2 69.2(4) 3 3
O20 Mo4 O7 104.6(2) . .
O20 Mo4 O11 91.0(3) . 3
O7 Mo4 O11 107.8(3) . 3
O20 Mo4 O11' 117.2(3) . 3
O7 Mo4 O11' 87.9(3) . 3
O11 Mo4 O11' 29.1(3) 3 3
O20 Mo4 O15' 111.2(5) . 3
O7 Mo4 O15' 142.2(5) . 3
O11 Mo4 O15' 83.9(3) 3 3
O11' Mo4 O15' 86.6(4) 3 3
O20 Mo4 O12 99.9(3) . .
O7 Mo4 O12 86.3(2) . .
O11 Mo4 O12 159.6(3) 3 .
O11' Mo4 O12 142.8(3) 3 .
O15' Mo4 O12 76.1(3) 3 .
O20 Mo4 O15 87.2(4) . 3
O7 Mo4 O15 164.7(3) . 3
O11 Mo4 O15 81.4(3) 3 3
O11' Mo4 O15 95.5(3) 3 3
O15' Mo4 O15 24.1(3) 3 3
O12 Mo4 O15 82.0(3) . 3
O20 Mo4 O1 154.5(2) . 3
O7 Mo4 O1 100.3(2) . 3
O11 Mo4 O1 76.0(3) 3 3
O11' Mo4 O1 57.9(3) 3 3
O15' Mo4 O1 46.5(5) 3 3
O12 Mo4 O1 87.1(2) . 3
O15 Mo4 O1 69.4(4) 3 3
O21 Mo5 O16' 117.5(6) . .
O21 Mo5 O12 102.1(3) . .
O16' Mo5 O12 92.2(4) . .
O21 Mo5 O8 100.3(2) . .
O16' Mo5 O8 141.3(5) . .
O12 Mo5 O8 87.5(2) . .
O21 Mo5 O16 89.8(4) . .
O16' Mo5 O16 27.7(3) . .
O12 Mo5 O16 100.1(3) . .
O8 Mo5 O16 165.9(4) . .
O21 Mo5 O13' 89.4(3) . .
O16' Mo5 O13' 84.7(3) . .
O12 Mo5 O13' 168.1(3) . .
O8 Mo5 O13' 87.8(3) . .
O16 Mo5 O13' 82.5(3) . .
O21 Mo5 O13 111.9(3) . .
O16' Mo5 O13 85.1(4) . .
O12 Mo5 O13 142.9(3) . .
O8 Mo5 O13 72.6(2) . .
O16 Mo5 O13 94.6(3) . .
O13' Mo5 O13 25.5(3) . .
O21 Mo5 O2 157.9(3) . .
O16' Mo5 O2 46.9(5) . .
O12 Mo5 O2 94.8(2) . .
O8 Mo5 O2 94.6(2) . .
O16 Mo5 O2 73.1(4) . .
O13' Mo5 O2 74.8(3) . .
O13 Mo5 O2 57.3(3) . .
O22 Mo6 O13 104.1(5) . .
O22 Mo6 O14 101.9(4) . .
O13 Mo6 O14 98.0(4) . .
O22 Mo6 O10 102.4(4) . .
O13 Mo6 O10 85.2(5) . .
O14 Mo6 O10 153.9(4) . .
O22 Mo6 O11 98.7(3) . .
O13 Mo6 O11 155.2(3) . .
O14 Mo6 O11 86.5(6) . .
O10 Mo6 O11 80.5(3) . .
O22 Mo6 O1 169.3(6) . .
O13 Mo6 O1 86.4(3) . .
O14 Mo6 O1 74.5(4) . .
O10 Mo6 O1 79.9(3) . .
O11 Mo6 O1 71.2(3) . .
O22 Mo6' O13' 102.7(4) . .
O22 Mo6' O14' 103.4(5) . .
O13' Mo6' O14' 97.6(4) . .
O22 Mo6' O10' 99.5(4) . .
O13' Mo6' O10' 87.2(6) . .
O14' Mo6' O10' 154.8(4) . .
O22 Mo6' O11' 101.6(5) . .
O13' Mo6' O11' 154.3(4) . .
O14' Mo6' O11' 84.8(5) . .
O10' Mo6' O11' 80.6(3) . .
O22 Mo6' O2 170.9(6) . .
O13' Mo6' O2 74.6(4) . .
O14' Mo6' O2 85.6(3) . .
O10' Mo6' O2 71.8(3) . .
O11' Mo6' O2 80.1(3) . .
C1 S1 C3 104.2(3) . .
C5 S2 C4 103.9(3) . .
N2 N1 N4 106.4(5) . .
N1 N2 N3 111.4(5) . .
N1 N2 Ag1 118.3(4) . .
N3 N2 Ag1 130.3(4) . .
C1 N3 N2 104.9(5) . .
C1 N3 Ag1 139.7(4) . 3_556
N2 N3 Ag1 115.4(4) . 3_556
N4 C1 N3 108.5(5) . .
N4 C1 S1 119.3(5) . .
N3 C1 S1 132.3(5) . .
N6 C5 N5 108.2(7) . .
N6 C5 S2 131.9(6) . .
N5 C5 S2 120.0(5) . .
C5 N6 N7 104.9(6) . .
C5 N6 Ag1 136.8(5) . 3_556
N7 N6 Ag1 118.2(4) . 3_556
N8 N7 N6 112.6(6) . .
N8 N7 Ag2 123.7(5) . .
N6 N7 Ag2 123.7(4) . .
N7 N8 N5 104.9(6) . .
P1 O1 O15' 142.9(5) . .
P1 O1 O4 48.4(3) . .
O15' O1 O4 112.8(5) . .
P1 O1 Mo2 125.8(3) . .
O15' O1 Mo2 47.8(3) . .
O4 O1 Mo2 77.6(3) . .
P1 O1 Mo4 123.3(3) . 3
O15' O1 Mo4 52.6(3) . 3
O4 O1 Mo4 148.9(4) . 3
Mo2 O1 Mo4 99.3(2) . 3
P1 O1 Mo6 120.1(4) . .
O15' O1 Mo6 96.9(5) . .
O4 O1 Mo6 121.5(4) . .
Mo2 O1 Mo6 89.2(3) . .
Mo4 O1 Mo6 89.1(2) 3 .
P1 O2 O16' 142.8(5) . .
P1 O2 O4 48.1(3) . 3
O16' O2 O4 110.3(5) . 3
P1 O2 O3 48.4(3) . .
O16' O2 O3 111.8(5) . .
O4 O2 O3 87.3(4) 3 .
P1 O2 Mo5 125.0(3) . .
O16' O2 Mo5 47.6(3) . .
O4 O2 Mo5 140.5(4) 3 .
O3 O2 Mo5 76.7(3) . .
P1 O2 Mo3 123.8(3) . 3
O16' O2 Mo3 53.5(3) . 3
O4 O2 Mo3 75.9(3) 3 3
O3 O2 Mo3 149.3(4) . 3
Mo5 O2 Mo3 100.0(3) . 3
P1 O2 Mo6' 119.8(4) . .
O16' O2 Mo6' 97.3(5) . .
O4 O2 Mo6' 129.4(4) 3 .
O3 O2 Mo6' 121.1(4) . .
Mo5 O2 Mo6' 89.2(3) . .
Mo3 O2 Mo6' 89.1(3) 3 .
O4 O3 P1 61.1(4) . .
O4 O3 O2 102.6(5) . .
P1 O3 O2 59.9(3) . .
O4 O3 Mo1 73.9(4) . .
P1 O3 Mo1 134.7(4) . .
O2 O3 Mo1 131.9(4) . .
O3 O4 P1 61.8(4) . .
O3 O4 O1 103.3(5) . .
P1 O4 O1 60.4(3) . .
O3 O4 O2 103.2(5) . 3
P1 O4 O2 60.2(3) . 3
O1 O4 O2 87.3(4) . 3
O3 O4 Mo1 73.4(4) . .
P1 O4 Mo1 134.9(4) . .
O1 O4 Mo1 131.6(4) . .
O2 O4 Mo1 141.0(4) 3 .
Mo1 O5 Mo2 140.2(3) . .
Mo3 O6 Mo1 140.1(3) . .
Mo4 O7 Mo1 140.0(3) . .
Mo1 O8 Mo5 138.7(3) . .
Mo2 O9 Mo3 138.6(2) . .
Mo3 O10 Mo6 151.6(4) 3 .
Mo4 O11 Mo6 123.2(4) 3 .
Mo6 O13 Mo5 150.2(4) . .
Mo6 O14 Mo2 121.3(4) . .
Mo3 O10' Mo6' 122.1(5) 3 .
Mo4 O11' Mo6' 151.2(5) 3 .
Mo6' O13' Mo5 121.0(5) . .
Mo6' O14' Mo2 151.3(5) . .
Mo5 O12 Mo4 140.4(2) . .
Mo2 O15 Mo4 117.0(6) . 3
Mo2 O15' O1 83.8(5) . .
Mo2 O15' Mo4 159.4(6) . 3
O1 O15' Mo4 80.9(5) . 3
Mo5 O16 Mo3 117.7(7) . 3
O2 O16' Mo5 85.6(6) . .
O2 O16' Mo3 81.0(5) . 3
Mo5 O16' Mo3 160.4(6) . 3
Mo6 O22 Mo6' 20.67(7) . .
C1 N4 N1 108.9(5) . .
C1 N4 C2 129.4(6) . .
N1 N4 C2 121.7(6) . .
C4 C3 S1 112.2(6) . .
C3 C4 S2 115.0(6) . .
C5 N5 N8 109.5(6) . .
C5 N5 C6 129.9(8) . .
N8 N5 C6 120.6(8) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ag1 N3 2.276(5) 3_556
Ag1 N6 2.282(6) 3_556
Ag1 N2 2.298(5) .
Ag2 N7 2.142(6) .
Ag2 N7 2.142(6) 3_656
P1 O4 1.423(7) .
P1 O4 1.423(7) 3
P1 O3 1.433(7) 3
P1 O3 1.433(7) .
P1 O1 1.653(6) .
P1 O1 1.653(6) 3
P1 O2 1.658(7) 3
P1 O2 1.658(7) .
Mo1 O17' 1.685(14) .
Mo1 O17 1.693(14) .
Mo1 O5 1.823(4) .
Mo1 O8 1.828(4) .
Mo1 O6 1.978(4) .
Mo1 O7 1.985(4) .
Mo1 O3 2.423(7) .
Mo1 O4 2.429(7) .
Mo2 O18 1.666(5) .
Mo2 O15' 1.720(8) .
Mo2 O9 1.805(4) .
Mo2 O5 1.978(5) .
Mo2 O15 1.981(10) .
Mo2 O14 2.007(7) .
Mo2 O14' 2.071(8) .
Mo2 O1 2.309(7) .
Mo3 O19 1.649(5) .
Mo3 O6 1.814(5) .
Mo3 O10' 1.839(8) 3
Mo3 O10 1.887(7) 3
Mo3 O16' 1.909(8) 3
Mo3 O9 2.010(4) .
Mo3 O16 2.185(10) 3
Mo3 O2 2.346(7) 3
Mo4 O20 1.656(5) .
Mo4 O7 1.815(5) .
Mo4 O11 1.829(7) 3
Mo4 O11' 1.888(8) 3
Mo4 O15' 1.903(8) 3
Mo4 O12 1.984(4) .
Mo4 O15 2.198(9) 3
Mo4 O1 2.366(7) 3
Mo5 O21 1.662(5) .
Mo5 O16' 1.716(8) .
Mo5 O12 1.808(4) .
Mo5 O8 1.981(5) .
Mo5 O16 1.987(10) .
Mo5 O13' 1.998(8) .
Mo5 O13 2.092(7) .
Mo5 O2 2.318(7) .
Mo6 O22 1.672(4) .
Mo6 O13 1.823(11) .
Mo6 O14 1.822(12) .
Mo6 O10 1.996(10) .
Mo6 O11 2.007(10) .
Mo6 O1 2.443(7) .
Mo6' O22 1.689(5) .
Mo6' O13' 1.836(13) .
Mo6' O14' 1.839(12) .
Mo6' O10' 1.993(12) .
Mo6' O11' 1.993(11) .
Mo6' O2 2.435(8) .
S1 C1 1.726(6) .
S1 C3 1.808(8) .
S2 C5 1.729(8) .
S2 C4 1.798(9) .
N1 N2 1.289(7) .
N1 N4 1.340(7) .
N2 N3 1.362(7) .
N3 C1 1.333(8) .
N3 Ag1 2.276(5) 3_556
C1 N4 1.334(8) .
C5 N6 1.316(8) .
C5 N5 1.344(10) .
N6 N7 1.362(8) .
N6 Ag1 2.282(6) 3_556
N7 N8 1.285(8) .
N8 N5 1.345(9) .
O1 O15' 1.738(15) .
O1 O4 1.801(9) .
O1 Mo4 2.366(7) 3
O2 O16' 1.697(16) .
O2 O4 1.814(9) 3
O2 O3 1.819(9) .
O2 Mo3 2.346(7) 3
O3 O4 1.366(10) .
O4 O2 1.814(9) 3
O10 Mo3 1.887(7) 3
O11 Mo4 1.829(7) 3
O10' Mo3 1.839(8) 3
O11' Mo4 1.888(8) 3
O15 Mo4 2.198(9) 3
O15' Mo4 1.903(8) 3
O16 Mo3 2.185(10) 3
O16' Mo3 1.909(8) 3
N4 C2 1.459(8) .
C3 C4 1.499(9) .
N5 C6 1.467(10) .
